Research Article  Open Access
Comprehensive Study on Elastic Moduli Prediction and Correlation of Glass and Glass Ceramic Derived from Waste Rice Husk
Abstract
Zinc silicate (ZnO–SiO_{2}) systems were fabricated using zinc oxide (ZnO) and white rice husk ash (WRHA) with compositions of (ZnO)_{x}(WRHA)_{1−x} ( = 0.55, 0.60, 0.65, and 0.70 wt.%) was symbolized by S1, S2, S3, and S4, respectively. The ZnO–SiO_{2} samples were fabricated by applying the meltquench method and the physical and elastic properties of the samples were investigated. Physical properties used in this study are density and molar volume while the theoretical elastic moduli of the samples produced were obtained using direct calculation of theoretical model compared with the experimental elastic moduli obtained by acquiring ultrasonic velocities using ultrasonic pulseecho technique. Values of experimental elastic moduli including longitudinal modulus (), shear modulus (), Young’s modulus (), bulk modulus (), and Poisson’s ratio () were compared with theoretical model calculated using Rocherulle’s model. All the configurations of the elastic moduli obtained experimentally match very well with the configuration from Rocherulle’s model but Poisson’s ratio obtained experimentally differs from the values of Poisson’s ratio obtained through Rocherulle’s model.
1. Introduction
Rice is the main source of carbohydrates and consumption for the populations in Asia and the main byproduct is the waste rice husk (RH) which is produced in a vast production of paddy field in Malaysia and also throughout the globe. Rice cultivation in Malaysia has resulted in 400,000 metric tonnes of RH annually as it has been considered valueless and the main problem arises once it comes to the problem of getting rid of it [1]. RH is obtained as a worthless byproduct as it cannot fetch a good price in the open market and most of the RH milling factories are massively influenced by this problem and disposing RH ethically will become unprofitable for them [2, 3]. RH produced is generally discarded or burned and this has caused a serious threat to our mother earth and by developing new ways to reuse RH, it can be a useful byproduct such as substitution for conventional silica in the glass industry [4, 5]. Next, substitution silica such as white rice husk ash (WRHA) can be derived from RH by a complete combustion [6]. RH serves as good substituents for conventional silica as it possesses high concentration of silica after complete combustion of 1000°C from WRHA and it has relatively lower cost compared to its conventional silica counterpart [7, 8]. RH glass system which is derived can be doped into lithium silicate glass system and it mimics the thermal behavior and crystalline phases of the glass and glass ceramic lithium silicate systems and it also increases the fracture toughness of both systems by 100% thus implying that RH will act as an adequate replacement for conventional silica [9]. RH glass ceramic can be used to derive nepheline–forsterite glass ceramic where its main source of silica is from WRHA [10].
Zinc silicate (ZnO–SiO_{2}) glass is an amorphous glass with high concentration of ZnO in its major composition and it grabs much attention from researches as it possesses various applicable uses in the range of glass ceramics and technical glasses [11]. Researchers can do a lot more to understand the applications of ZnO–SiO_{2} glass and by variating SiO_{2} and ZnO compositions, endless possibilities can be achieved. ZnO is one of the major compositions in the samples produced and incorporating it in the glass and glass ceramic system makes ZnO–SiO_{2} system a remarkable one. ZnO based glass is one of the most interesting network modifiers in the list of all the network modifiers because of its influence in the optical, electrical, and magnetic properties of the glass produced causing the glass to be environmentfriendly and of low cost which grabs the attention of researches and manufacturing industry [12, 13]. Silicate glass doped with high concentration of ZnO has lower elastic moduli because of the effect presented by ZnO which acts as a network modifier and its effect is what causes these types of glass to be outstanding compared to other types of glass system [14].
In this study, ZnO and WRHA will be manipulated to study the physical and elastic properties of ZnO–SiO_{2} glass and glass ceramic system. Influence of ZnO on its elastic moduli and comparison of elastic moduli obtained experimentally and elastic moduli obtained theoretically were also discussed.
2. Experimental Details
RH species used is the Oryza sativa (Asian rice) which can be found in majority of Asian countries and RH from this study is acquired from a local rice factory at Tanjung Karang, Selangor, Malaysia. RH samples used were just milled a day before the study and they are kept in an indoor compound to minimize possible unwanted contaminations from the surroundings. RH then is examined to remove sands and small rocks which jeopardize the study. Next, RH is then washed for several times to get rid of possible dirt and contaminations as it is in contact with sand and it is drenched in water for 2 hours in a vast plastic basin to have the dirt and sands sunken to the bottom of the plastic basin. RH which is clean and clear without contaminations will float on the surface and it is removed to a large plastic sieve to dry the RH with an aluminum foil on top of it to minimize contaminations from the surroundings as it will be left in the lab for 24 hours to dry at room temperature. After 24 hours, RH will be subsequently dried in the oven for 2 hours at 100°C for 24 hours to obtain a fully dried RH. After obtaining the dry RH, 500 g of the dried RH is transferred to a ceramic crucible and distributed evenly so that the combustion of RH to WRHA can be performed evenly. RH will be burned at 1000°C for 2 hours at a heating rate of 10°C/min and the changes in color of the WRHA produced are observed. Ceramic crucible selected must be flat as it delivers a complete homogeneous burning of RH. The EDXRF measurement has been done to obtain the percentage of the oxide composition in the WRHA [16].
In this study WRHA is acquired to replace conventional silica in the formation of ZnO–SiO_{2} glass and glass ceramic system chemical formula of (ZnO)_{x}(WRHA)_{1−x} ( = 0.55, 0.60, 0.65, and 0.70 wt.%) was symbolized by S1, S2, S3, and S4, respectively, acquiring meltquench technique. After mixing the samples, the mixture is then milled for 24 hours to ensure a fully homogenous mixture. Usually, melting silicate glass system would require up to 1700°C as it belongs to type of glass with high melting point but in this study, where the silica source is being manipulated by switching it to WRHA to form ZnO–SiO_{2} glass system, a new method is being done with the lowest temperature at which ZnO–SiO_{2} system can exist at 1450°C with 2 hours. After all the samples inside the crucible were successfully melted, the crucible was removed with a platinum clamp and the samples are transferred to a stainless steel mold which has been preheated at 500°C and the samples then are annealed at 500°C for 5 hours while the leftover samples were transferred into the same stainless steel base which holds the mold and is annealed at the similar condition. Finally the samples were cut using a diamond blade cutter to a dimension of (1.0 × 2.0 × 0.3) cm^{3} and later the samples were grinded using several grinding papers in the range of 320–1000 grit to ensure a perfect smooth surface for ultrasonic measurement. Samples thickness of (1.0 × 2.0 × 0.3) cm^{3} is the optimum thickness because samples which are too thick or too thin may cause the decrease in ultrasonic wave intensity.
The compositions of the glass and glass ceramic samples are confirmed using EDXRF diffractometer (Shimadzu, EDX720). Next, the densities of the samples were determined using the Archimedes method where it acquires the weight of the samples in air and distilled water. Based on the Archimedes method, the buoyant force produced when the sample is immersed in distilled water is the same with the magnitude of the weight of distilled water displaced by the volume of the samples. Hence, the density of samples, , can be expressed aswhere g cm^{−3}. Distilled water was chosen as the immersed liquid as it is the cheap, inert, and low surface tension. Molar volume () of any substance is defined as the volume occupied by one mole of any material from chemical compound or chemical element at a specified temperature and pressure formula of is equal to the total molar mass () divided by the mass density ().
The molar volumes were measured in cubic centimeters per mole (cm^{3} mol^{−1}) and for liquids and solids; they can be expressed aswhere is the total molecular weight of the multicomponent system given bywhere is the mole fraction of the th oxides, and is the molecular weight of the th oxides. Ultrasonic velocities of the samples which consist of longitudinal velocity () and shear velocity () were determined using Ritec, Ram5000 Snap System machine with frequency of 5 MHz. Longitudinal velocity of the samples was acquired using the longitudinal probe while the shear velocity of the samples was acquired using the shear probe. Adhesive agent used for the longitudinal probe is longitudinal gel while the shear probe is shear gel. Adhesive agent is used to minimize the refraction of wave in air gap while acquiring both ultrasonic velocities.
Ultrasonic technique is a method that is useful and flexible to measure the structure and mechanical properties of materials. Next, ultrasonic waves can be transmitted through the material and detect the mechanical properties and the defects found in the material. Generally, ultrasonic measurement can be used to measure the metal and nonmetal samples. Ultrasonic pulseecho technique can also be known as the longitudinal modulus and shear modulus.
3. Results and Discussion
Four series of ZnO–SiO_{2} samples were obtained and chemical composition of the WRHA was analyzed using EDXRF and the chemical composition of the WRHA and samples produced was tabulated in Table 1.

Figure 1 and Table 2 show the density, molecular weight, and molar volume for ZnO–SiO_{2} samples and it shows that the density of the samples increases with the increase of ZnO from 2.94 to 3.66 g cm^{−1}. Increase in density is largely due to substituting Si (28.08) with a higher atomic mass element of zinc which is (65.39). Besides, the increase in density with the increase of ZnO content occurs due to the increase in the crystallinity in the samples in which sample S1 is fully amorphous and sample S4 provides higher amounts of crystalline compared to the other samples [17, 18]. Increase in crystallinity is due to the increase in melting point of the ZnO–SiO_{2} samples as its melting point increases as ZnO in the system increases as shown in Figure 2. Not only that, silica present in the system will also act as a nucleating agent for the samples to increase in crystalline [15].

Increase in density can also be explained by the increase in ZnO and the reduction of silica (SiO_{2}) which will increase its overall molecular weight of the samples as ZnO is much heavier relative to molecular mass of SiO_{2} [19]. Increase in density of the ZnO–SiO_{2} samples may also be caused by structural reorganization of the atoms thus causing a possible modification of the geometrical configuration.
Molar volume () in this study was calculated using (2) and, based on Figure 1 and Table 2, molar volumes of the ZnO–SiO_{2} samples produced indicate a decrease from 23.97 to 20.18 cm^{3} mol^{−1} when the amount of ZnO in the samples increases. Molar volume is vastly dependent on the overall molecular weight of a particular composition and this decrease is mainly because of greater rise in density compared to the overall molecular weight. Generally, silicate glass and glass ceramic have an opposite trend to the density of its system when it comes to the molar volume and, in this study, SiO^{2+} (0.038 nm) which is greater in ionic radius is substituted with Zn^{2+} (0.074 nm) thus causing the increase in the interatomic spacing or bond length between the atoms [20]. Besides that, the overall reduction in the interatomic distances will result in the increase of compactness of the glass matrix [21].
Decrease in can also be attributed to the addition of ZnO as it causes some kind of structural rearrangement of the atoms by entering the glass system and destroying the Si–O–Si bonds, thus creating ionic bonds between Zn^{2+} and single bonded oxygen atoms [20]. Next, there is also a possibility for the modification of the geometrical configuration upon swapping ZnO into the glass network and the structure of the studied glasses will not be expanded, which have more compact and low number of covalent bonds with high reduction in the number of bridging oxygens (BOs) [22]. Longitudinal velocity () and the shear velocity () of the samples were acquired and are presented in Table 3 and were plotted in Figure 3. Generally, and of majority of materials will increase as the density of the system increases but, for this study, and decrease as the density of the system increases. Similar trends were also observed for soda lime silicate and silicate glass system whereby the and of the samples decrease when the density in the sample increases [23]. Decrease in and of the samples is due to rise in amount of ZnO present in the samples which contains Zn^{2+} ions where its zinc atom had higher atomic radius compared to Si atom therefore encouraging the transformation of BOs to NBOs in the system.

Based on Table 3, values of are much smaller compared to the value of its counterpart and it can be considered half of the value of at the same compositions. For example, sample S1 which has a value of is 1951.95 ms^{−1} while its is 3857.03 ms^{−1} which shows that its shear velocity is half of the longitudinal velocity and the trend is constant throughout all samples. Next, the values of decrease from 3857.03 ms^{−1} to 2482.31 ms^{−1} while decreases from 1951.95 ms^{−1} to 966.27 ms^{−1} as the amount of ZnO increases. Increase in the amount of ZnO in the samples promotes the formation of NBOs and it is because ZnO which acts as a network former and Zn^{2+} ions are the main result which causes the increase in NBOs. In the glass system, average coordination number of SiO_{2} gradually reduced to 3 from 4 as the values of ZnO rise and this causes the structural units of SiO_{4} to be converted to SiO_{3} initiating the rise of NBOs [24–26]. Decrease in both and with the rise of ZnO also indicates that the ultrasonic wave encounters more resistance in the ZnO–SiO_{2} samples as the amount of ZnO increases [27, 28]. Not only that, rise of ZnO in the ZnO–SiO_{2} samples also indicates that more Zn^{2+} ions exist in the samples and this caused overall more ions in samples to be opened up [29]. A result of lower ultrasonic velocity at higher content of ZnO indicates a major alteration in the structures of the samples.
Experimental values of longitudinal modulus (), shear modulus (), Young’s modulus (), bulk modulus (), Poisson’s ratio (), fractal bond connectivity (), and microhardness () were calculated from the data obtained by ultrasonic velocities. The results of the elastic properties of the ZnO–SiO_{2} samples are shown in Table 4. As seen, from Table 4, all the values of the elastic moduli decrease with the rise in ZnO.

Longitudinal modulus and shear modulus can be defined as an independent elastic constant which are produced by a small stress such as the elastic strain in an amorphous solid [30]. Longitudinal modulus is and for pure shear modulus it is , where and , respectively, are the longitudinal and shear velocities of the samples [31]. The longitudinal modulus (), shear modulus (), Young’s modulus (), bulk modulus (), Poisson’s ratio (), and microhardness can be obtained using the ultrasonic velocities by acquiring these equations from the following journals by Laoding et al. (2016) and Sidek et al. (2016) [32, 33]. Based on Table 4 and Figure 4 which illustrate the values and plot of longitudinal modulus and shear modulus of the ZnO–SiO_{2} samples, it can be seen that as the amount of ZnO in the samples increases, the longitudinal modulus and shear modulus decrease. Decrease in longitudinal modulus from samples S1 to S4 is from 43.74 GPa to 22.54 GPa while decrease in shear modulus from samples S1 to S4 is from 11.20 GPa to 3.42 GPa. Longitudinal modulus for every sample is higher compared to its counterpart of shear modulus for every sample from S1 to S4 and this implies that the sample can withstand longitudinal stress compared to shear stress which indicates the samples are easier to be bent than elongated.
Young’s modulus is defined as the ratio of stress against strain and it also represents the stiffness in a particular material which links to bonding strength between atoms in materials. Materials which have higher value of Young’s modulus imply that that particular material is more stiffer and this Young’s modulus is also affected by the dimensionality and connectivity of the system [33]. Not only that, samples that have higher value of Young’s modulus can endure more stress compared to samples which possess lower Young’s modulus and Figure 5 shows that as the amount of ZnO in the samples increases, Young’s modulus of the samples decreases which indicates the increase in number of NBOs [34]. Decrease in the NBOs further links to the decrease in connectivity of the samples network which is caused by the decrease in Young’s modulus. Lower Young’s modulus as ZnO increases shows that the ZnO–SiO_{2} samples can reduce the speed of impacting mass thus causing a smaller stress compared to samples which have higher Young’s modulus [34]. Results of Young’s modulus can indicate that the samples can bear small stress acting against it even though its structure is less rigid and the decrease in Young’s modulus indicates that the samples can work well with strain.
Bulk modulus () is known as the alteration in volume of a material when a small or moderate force is performed upon the specific surface. Figure 6 shows that as the amount of ZnO in the system increases, the bulk modulus of the samples increases and the bulk modulus of the samples is higher compared to Young’s modulus which indicates that the samples work well with stress from multiple directions but not in one direction. Hence this clearly means that glass and glass ceramic acquired are usually hard if stress is applied from numerous directions simultaneously but would fracture if stress is applied at a single direction. Bergman and Kantor (1984) proposed the analysis of fractal bond connectivity with ratio of bulk to shear modulus and it can be simplified as where it gives the effective dimensionality of particular materials for any nonhomogeneous random mixture of fluid and a solid backbone near the percolation limit [35]. Value of acts as a parameter for network connectivity with a range of values obtained by the ratio [36]. Values of differ for each kind of materials subjected on its dimension and d = 1 is for 1D chain and and for 2D and 3D chain structures correspondingly [37–39]. Results shown in Figure 7 and Table 4 indicate that the fractal bond connectivity of the ZnO–SiO_{2} samples ranges from 0 to 1 which shows that ZnO–SiO_{2} samples possess a 1D layer structure [40]. As ZnO increases in the samples, fractal bond connectivity decreases and this will cause crosslinks of the samples to be weakened and possibly break [23].
Poisson ratio is the measure of ratio of the shear strain to the longitudinal strain when tensile force is applied and it makes use of the degree of crosslink density of glass and glass ceramic network to find out the order of crosslink density [41]. Poisson’s ratio measures the capability of a material to counter the alteration in volume when an incoming load acts on a certain material and the Poisson ratio (v) acquired can be in positive or negative [42]. In this study it is in the range of 0.327 to 0.410.
From Figure 8, it is observed that, as ZnO increases in the samples, results in higher values of Poisson’s ratio show that the samples have a lower resistance towards lateral expansion when compressed compared to samples with lower amount of ZnO. Rise in Poisson’s ratio also shows that the decrease in crosslink density and lateral strength with the increase in ZnO as network former does not have much significance in its crosslink density [43]. Relationship between Poisson’s ratio and crosslink density was first discussed by Bridge et al. (1983) and its relationship is known as the number of bridging bonds per cations in the structure of the system where results of the crosslink density 0, 1, and 2 are associated with the values of Poisson’s ratio obtained, 0.40, 0.30, and 0.15, correspondingly [44]. Average value of Poisson’s ratio acquired in these samples is 0.34 which suggests that the samples have 1D layer structure and values of this result correlate with the results from fractal bond connectivity which is around 1.
Microhardness () is known to be the total stress which is necessary to remove the free volume or distortion of the glass and glass ceramic network [45]. Based on Figure 9, the microhardness of the samples decreases as the amount of ZnO increases in the system and indicates a decrease in the connectivity of the glass and glass ceramic system. Application of hydrostatic pressure is necessary to decrease the free volume in the glass and glass ceramic system [46].
After completing experimental elastic moduli, it is always interesting to predict the results of elastic moduli without performing experimental methods. Theory of elastic prediction has been brought up by Makishima and Mackenzie (1973, 1975) on the prediction of elastic moduli of oxide glass by utilizing composition of oxides and packing density of chemical composition of the glass [47, 48].
Rocherulle et al. (1989) improved the packing density of the equation approximately 20 years later and incorporated aswhere and are Pauling’s ionic radius of cation A and anions O, and are the density and effective molecular weight, and is the new packing density [49]. This model offers a new derivation of elastic moduli and Poisson ratio’s for the current system aswhere , , , and are the total packing density, total dissociation energy per unit volume, dissociation energy per unit volume, and the mole fraction of the oxide th component correspondingly.
Table 5 illustrates the theoretical calculated total packing density, , longitudinal modulus, , shear modulus, , Young’s modulus, , bulk modulus, , and Poisson’s ratio, , based on Rocherulle’s model. Based on the values of theoretical elastic moduli and Poisson’s ratio of ZnO–SiO_{2} samples obtained, it can be observed that the all the theoretical elastic moduli and Poisson’s ratio decrease when composition of ZnO increases. Longitudinal modulus calculated decreases from 46.53 GPa to 40.93 GPa, shear modulus decreases from 15.57 GPa to 13.88 GPa, Young’s modulus decreases from 36.83 GPa to 32.71 GPa, bulk modulus decreases from 25.78 GPa to 22.42 GPa, and Poisson’s ratio decreases from 0.2626 to 0.2576. Decrease in elastic moduli and Poisson’s ratio as ZnO increases suggests that ZnO would act as network modifier thus breaking BOs and converts it to NBOs which will decrease the connectivity and elastic moduli of the samples. Elastic moduli and Poisson’s ratio predicted by using Rocherulle’s model were illustrated in Figures 10 and 11. Comparisons of the experimental elastic moduli and Poisson’s ratio and the theoretical elastic moduli and Poisson’s ratio were illustrated in Figures 12–16. Experimental elastic moduli and theoretical elastic moduli have a great agreement in similar trend but vary in value except for Poisson’s ratio.

4. Conclusion
(ZnO)_{x}(WRHA)_{1−x} ( = 0.55, 0.60, 0.65 and 0.70 wt.%) was symbolized by S1, S2, S3, and S4, respectively, samples have been successfully fabricated, and the study of elastic moduli with prediction of its correlation with the variation of composition on physical and elastic characteristics of each sample was performed and analyzed. Physical analysis of the samples shows that as ZnO increases, the density of the overall samples decreases and this is very well associated with the formation of NBOs and its molar volume increases as ZnO increase which is caused by the substitution of ions of Zn^{2+} which is greater in interatomic spacing compared to SiO^{2+}. Last but not least, all the theoretical elastic moduli possess the same trend as the elastic moduli obtained experimentally suggesting that ZnO would act as network modifier thus breaking BOs and converts it to NBOs which will decrease the connectivity and elastic moduli of the samples.
Conflicts of Interest
The authors declare that there are no conflicts of interest regarding the publication of this paper.
Acknowledgments
The researchers gratefully acknowledge the financial support for this study from the Malaysian Ministry of Higher Education (MOHE) and Universiti Putra Malaysia through the Fundamental Research Grant Scheme (FRGS) and Geran Putra Berimpak research grant.
References
 A. M. Yusof, N. A. Nizam, and N. A. A. Rashid, “Hydrothermal conversion of rice husk ash to faujasitetypes and NaAtype of zeolites,” Journal of Porous Materials, vol. 17, no. 1, pp. 39–47, 2010. View at: Publisher Site  Google Scholar
 M. Ahmaruzzaman and V. K. Gupta, “Rice husk and its ash as lowcost adsorbents in water and wastewater treatment,” Industrial & Engineering Chemistry Research, vol. 50, no. 24, pp. 13589–13613, 2011. View at: Google Scholar
 O. Mohiuddin, A. Mohiuddin, M. Obaidullah, H. Ahmed, and S. AsumaduSarkodie, “Electricity production potential and social benefits from rice husk, a case study in Pakistan,” Cogent Engineering, vol. 3, no. 1, Article ID 1177156, 2016. View at: Publisher Site  Google Scholar
 M. Arabani, S. A. Tahami, and M. Taghipoor, “Laboratory investigation of hot mix asphalt containing waste materials,” Road Materials and Pavement Design, vol. 18, no. 3, pp. 713–729, 2017. View at: Publisher Site  Google Scholar
 S. Kamari and F. Ghorbani, “Synthesis of magMCM41 with rice husk silica as cadmium sorbent from aqueous solutions: parameters’ optimization by response surface methodology,” Environmental Technology (United Kingdom), pp. 1–18, 2016. View at: Publisher Site  Google Scholar
 S. A. Saad, M. F. Nuruddin, N. Shafiq, and M. Ali, “The effect of incineration temperature to the chemical and physical properties of ultrafine treated rice husk ash (UFTRHA) as supplementary cementing material (SCM),” in Proceedings of the 4th International Conference on Process Engineering and Advanced Materials, ICPEAM 2016, pp. 163–167, Kuala Lumpur, Malaysia, August 2016. View at: Google Scholar
 B. O. Ayomanor and K. VernonParry, “Potential synthesis of solargrade silicon from rice husk ash,” Solid State Phenomena, vol. 242, pp. 41–47, 2016. View at: Publisher Site  Google Scholar
 I. J. Fernandes, D. Calheiro, A. G. Kieling et al., “Characterization of rice husk ash produced using different biomass combustion techniques for energy,” Fuel, vol. 165, pp. 351–359, 2016. View at: Publisher Site  Google Scholar
 F. A. Santos, C. dos Santos, D. Rodrigues Junior et al., “Lithium disilicate glassceramic obtained from rice huskbased silica,” Advances in Science and Technology, vol. 63, no. 1, pp. 414–419, 2010. View at: Google Scholar
 M. I. Martín, F. Andreola, L. Barbieri et al., “Crystallisation and microstructure of nepheline–forsterite glassceramics,” Ceramics International, vol. 39, no. 3, pp. 2955–2966, 2013. View at: Google Scholar
 M. H. M. Zaid, K. A. Matori, H. A. A. Sidek et al., “Fabrication and crystallization of ZnOSLS glass derived willemite glassceramics as a potential material for optics applications,” Journal of Spectroscopy, vol. 2016, Article ID 8084301, 2016. View at: Publisher Site  Google Scholar
 X. L. Duan, D. R. Yuan, D. Xu et al., “Preparation and characterization of Co^{2+}doped ZnOAl_{2}O_{3}SiO_{2} glassceramics by the sol–gel method,” Materials research bulletin, vol. 38, no. 4, pp. 705–711, 2003. View at: Google Scholar
 L. Yu and M. Nogami, “Local structure and photoluminescent characteristics of Eu^{3+} in ZnOSiO_{2} glasses,” Journal of SolGel Science and Technology, vol. 43, no. 3, pp. 355–360, 2007. View at: Publisher Site  Google Scholar
 K. A. Matori, M. H. M. Zaid, H. A. A. Sidek, M. K. Halimah, Z. A. Wahab, and M. G. M. Sabri, “Influence of ZnO on the ultrasonic velocity and elastic moduli of soda lime silicate glasses,” International Journal of Physical Sciences, vol. 5, no. 14, pp. 2212–2216, 2010. View at: Google Scholar
 E. N. Bunting, “Phase equilibria in the system SiO_{2}–ZnO,” Journal of the American Ceramic Society, vol. 13, no. 1, pp. 5–10, 1930. View at: Publisher Site  Google Scholar
 A. J. A. AlNidawi, K. A. Matori, A. Zakaria, and M. H. M. Zaid, “Effect of MnO_{2} doped on physical, structure and optical properties of zinc silicate glasses from waste rice husk ash,” Results in Physics, vol. 7, pp. 955–961, 2017. View at: Publisher Site  Google Scholar
 S. Zhang and A. Stamboulis, “Effect of zinc substitution for calcium on the crystallisation of calcium fluoroaluminosilicate glasses,” Journal of NonCrystalline Solids, vol. 432, pp. 300–306, 2016. View at: Publisher Site  Google Scholar
 L. Chen and Y. Dai, “Structure, physical properties, crystallization and sintering of ironcalciumaluminosilicate glasses with different amounts of ZnO,” Journal of NonCrystalline Solids, vol. 452, pp. 45–49, 2016. View at: Publisher Site  Google Scholar
 M. H. M. Zaid, K. A. Matori, H. J. Quah et al., “Investigation on structural and optical properties of SLS–ZnO glasses prepared using a conventional melt quenching technique,” Journal of Materials Science: Materials in Electronics, vol. 26, no. 6, pp. 3722–3729, 2015. View at: Publisher Site  Google Scholar
 K. A. Matori, M. H. M. Zaid, H. J. Quah, H. A. A. Sidek, Z. A. Wahab, and M. G. M. Sabri, “Studying the effect of ZnO on physical and elastic properties of (ZnO)_{x}(P_{2}O_{5})_{1x} glasses using nondestructive ultrasonic method,” Advances in Materials Science and Engineering, vol. 2015, Article ID 596361, 2015. View at: Publisher Site  Google Scholar
 S. Y. Marzouk and M. S. Gaafar, “Ultrasonic study on some borosilicate glasses doped with different transition metal oxides,” Solid State Communications, vol. 144, no. 1011, pp. 478–483, 2007. View at: Publisher Site  Google Scholar
 H. A. Saudi, H. A. Sallam, and K. Abdullah, “Borosilicate glass containing bismuth and zinc oxides as a hot cell material for gammaray shielding,” Physics and Materials Chemistry, vol. 2, no. 1, pp. 20–24, 2014. View at: Google Scholar
 M. H. M. Zaid, K. A. Matori, L. C. Wah et al., “Elastic moduli prediction and correlation in soda lime silicate glasses containing ZnO,” International Journal of Physical Sciences, vol. 6, no. 6, pp. 1404–1410, 2011. View at: Google Scholar
 N. A. Sharaf, R. A. Condrate Sr., and A. A. Ahmed, “FTIR spectral/structural investigation of the ion exchange/thermal treatment of silver ions into a silicate glass,” Materials Letters, vol. 11, no. 34, pp. 115–118, 1991. View at: Publisher Site  Google Scholar
 P. F. Wang, Z. H. Li, J. Li, and Y. M. Zhu, “Effect of ZnO on the interfacial bonding between Na_{2}OB_{2}O_{3}SiO_{2} vitrified bond and diamond,” Solid State Sciences, vol. 11, no. 8, pp. 1427–1432, 2009. View at: Publisher Site  Google Scholar
 A. Bernasconi, M. Dapiaggi, A. Pavese, G. Agostini, M. Bernasconi, and D. T. Bowron, “Modeling the structure of complex aluminosilicate glasses: The effect of zinc addition,” Journal of Physical Chemistry B, vol. 120, no. 9, pp. 2526–2537, 2016. View at: Publisher Site  Google Scholar
 Y. B. Saddeek, E. R. Shaaban, K. A. Aly, and I. M. Sayed, “Characterization of some lead vanadate glasses,” Journal of Alloys and Compounds, vol. 478, no. 12, pp. 447–452, 2009. View at: Publisher Site  Google Scholar
 M. M. Umair and A. K. Yahya, “Elastic and structural changes of xNa_{2}O–(35 − x)V_{2}O_{5}–65TeO_{2} glass system with increasing sodium,” Materials Chemistry and Physics, vol. 142, no. 23, pp. 549–555, 2013. View at: Publisher Site  Google Scholar
 K. A. Matori, M. I. Sayyed, H. A. A. Sidek, M. H. M. Zaid, and V. P. Singh, “Comprehensive study on physical, elastic and shielding properties of lead zinc phosphate glasses,” Journal of NonCrystalline Solids, vol. 457, pp. 97–103, 2017. View at: Publisher Site  Google Scholar
 C. Bootjomchai, “Comparative studies between theoretical and experimental of elastic properties and irradiation effects of soda lime glasses doped with neodymium oxide,” Radiation Physics and Chemistry, vol. 110, pp. 96–104, 2015. View at: Publisher Site  Google Scholar
 C. Weigel, C. Le Losq, R. Vialla et al., “Elastic moduli of XAlSiO_{4} aluminosilicate glasses: effects of chargebalancing cations,” Journal of NonCrystalline Solids, vol. 447, pp. 267–272, 2016. View at: Publisher Site  Google Scholar
 H. Laoding, H. Mohamed Kamari, A. Zakaria, A. H. Shaari, and I. Mansor, “Elastic properties of thulium doped zinc borotellurite glass,” Materials Science Forum, vol. 863, pp. 70–74, 2016. View at: Publisher Site  Google Scholar
 H. A. A. Sidek, R. ElMallawany, K. A. Matori, and M. K. Halimah, “Effect of PbO on the elastic behavior of ZnO–P_{2}O_{5} glass systems,” Results in Physics, vol. 6, pp. 449–455, 2016. View at: Publisher Site  Google Scholar
 R. A. Mccauley, A. K. De, and D. S. Carr, “Improved impact resistance in sodalimesilica glasses through zinc oxide substitutions,” Journal of the American Ceramic Society, vol. 64, no. 11, pp. 157158, 1981. View at: Publisher Site  Google Scholar
 D. J. Bergman and Y. Kantor, “Critical properties of an elastic fractal,” Physical Review Letters, vol. 53, no. 6, pp. 511–514, 1984. View at: Publisher Site  Google Scholar  MathSciNet
 K. Shinozaki, T. Honma, and T. Komatsu, “Elastic properties and Vickers hardness of optically transparent glassceramics with fresnoite Ba_{2}TiSi_{2}O_{8} nanocrystals,” Materials Research Bulletin, vol. 46, no. 6, pp. 922–928, 2011. View at: Publisher Site  Google Scholar
 R. Bogue and R. J. Sladek, “Elasticity and thermal expansivity of (AgI)_{x}(AgPO_{3})_{1−x} glasses,” Physical Review B, vol. 42, no. 8, pp. 5280–5288, 1990. View at: Publisher Site  Google Scholar
 G. A. Saunders, T. Brennan, M. Acet et al., “Elastic and nonlinear acoustic properties and thermal expansion of cerium metaphosphate glasses,” Journal of NonCrystalline Solids, vol. 282, no. 23, pp. 291–305, 2001. View at: Publisher Site  Google Scholar
 N. Ghribi, M. DutreilhColas, J.R. Duclère et al., “Structural, mechanical and optical investigations in the TeO_{2}rich part of the TeO_{2}GeO_{2}ZnO ternary glass system,” Solid State Sciences, vol. 40, pp. 20–30, 2015. View at: Publisher Site  Google Scholar
 A. Abd ElMoneim, “Correlation between acoustical and structural properties of glasses: Extension of Abd ElMoneim model for bioactive silica based glasses,” Materials Chemistry and Physics, vol. 173, pp. 372–378, 2016. View at: Publisher Site  Google Scholar
 L. A. El Latif, “Ultrasonic study on the role of Na_{2}O on the structure of Na_{2}OB_{2}O_{3} and Na_{2}OB_{2}O_{3}SiO_{2} glasses,” Journal of Pure and Applied Ultrasonic, vol. 27, no. 23, pp. 80–91, 2005. View at: Google Scholar
 G. N. Greaves, A. L. Greer, R. S. Lakes, and T. Rouxel, “Poisson's ratio and modern materials,” Nature Materials, vol. 10, no. 11, pp. 823–837, 2011. View at: Publisher Site  Google Scholar
 N. B. Mohamed, A. K. Yahya, M. S. M. Deni, S. N. Mohamed, M. K. Halimah, and H. A. A. Sidek, “Effects of concurrent TeO_{2} reduction and ZnO addition on elastic and structural properties of (90 − x)TeO_{2}–10Nb_{2}O_{5}–(x)ZnO glass,” Journal of NonCrystalline Solids, vol. 356, no. 3334, pp. 1626–1630, 2010. View at: Publisher Site  Google Scholar
 B. Bridge, N. D. Patel, and D. N. Waters, “On the elastic constants and structure of the pure inorganic oxide glasses,” Physica Status Solidi (A), vol. 77, no. 2, pp. 655–668, 1983. View at: Publisher Site  Google Scholar
 N. Sasmal, M. Garai, and B. Karmakar, “Influence of Ce, Nd, Sm and Gd oxides on the properties of alkalineearth borosilicate glass sealant,” Journal of Asian Ceramic Societies, vol. 4, no. 1, pp. 29–38, 2016. View at: Google Scholar
 T. Rouxel, “Driving force for indentation cracking in glass: composition, pressure and temperature dependence,” Philosophical Transactions of the Royal Society A: Mathematical, Physical and Engineering Sciences, vol. 373, no. 2038, Article ID 20140140, 2015. View at: Publisher Site  Google Scholar
 A. Makishima and J. D. Mackenzie, “Direct calculation of Young's moidulus of glass,” Journal of NonCrystalline Solids, vol. 12, no. 1, pp. 35–45, 1973. View at: Publisher Site  Google Scholar
 A. Makishima and J. D. Mackenzie, “Calculation of bulk modulus, shear modulus and Poisson's ratio of glass,” Journal of NonCrystalline Solids, vol. 17, no. 2, pp. 147–157, 1975. View at: Publisher Site  Google Scholar
 J. Rocherulle, C. Ecolivet, M. Poulain, P. Verdier, and Y. Laurent, “Elastic moduli of oxynitride glasses. Extension of Makishima and Mackenzie's theory,” Journal of NonCrystalline Solids, vol. 108, no. 2, pp. 187–193, 1989. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2017 Chee Sun Lee et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.